DOI: 10.17188/1740242
title: Materials Data on Li3MnV(PO4)3 by Materials Project

description: Li3VMn(PO4)3 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.77 Å. In the second Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 2.01–2.57 Å. In the third Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.01 Å. In the fourth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.00 Å. In the fifth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.54 Å. In the sixth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.76 Å. In the seventh Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.77 Å. In the eighth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.53 Å. In the ninth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.92–2.00 Å. In the tenth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–1.98 Å. In the eleventh Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.52 Å. In the twelfth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.74 Å. There are four inequivalent V4+ sites. In the first V4+ site, V4+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.95–2.19 Å. In the second V4+ site, V4+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.93–2.12 Å. In the third V4+ site, V4+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.91–2.12 Å. In the fourth V4+ site, V4+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.93–2.23 Å. There are four inequivalent Mn2+ sites. In the first Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.94–2.32 Å. In the second Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.90–2.20 Å. In the third Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.88–2.18 Å. In the fourth Mn2+ site, Mn2+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.92–2.35 Å. There are twelve inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 28–41°. There is one shorter (1.54 Å) and three longer (1.55 Å) P–O bond length. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 13–45°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 13–44°. There are a spread of P–O bond distances ranging from 1.50–1.57 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 16–47°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 11–44°. There are a spread of P–O bond distances ranging from 1.51–1.57 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 31–39°. There is one shorter (1.54 Å) and three longer (1.55 Å) P–O bond length. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 30–39°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 13–46°. There are a spread of P–O bond distances ranging from 1.51–1.59 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 17–45°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one VO6 octahedra and corners with three MnO6 octahedra. The corner-sharing octahedra tilt angles range from 11–46°. There are a spread of P–O bond distances ranging from 1.52–1.58 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 21–48°. There are a spread of P–O bond distances ranging from 1.54–1.57 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 31–37°. There is one shorter (1.53 Å) and three longer (1.55 Å) P–O bond length. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V4+, and one P5+ atom. In the second O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V4+, and one P5+ atom. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V4+, and one P5+ atom. In the fourth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+, one V4+, and one P5+ atom. In the sixth O2- site, O2- is bonded in a linear geometry to one V4+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a distorted rectangular see-saw-like geometry to two Li1+, one V4+, and one P5+ atom. In the ninth O2- site, O2- is bonded in a distorted tetrahedral geometry to two Li1+, one V4+, and one P5+ atom. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V4+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a linear geometry to one Mn2+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a linear geometry to one V4+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V4+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a distorted rectangular see-saw-like geometry to two Li1+, one V4+, and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a linear geometry to one V4+ and one P5+ atom. In the twentieth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V4+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V4+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V4+, and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+, one V4+, and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a linear geometry to one Mn2+ and one P5+ atom. In the thirty-first O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form a mixture of distorted edge and corner-sharing OLi2MnP trigonal pyramids. In the thirty-second O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-third O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form a mixture of distorted edge and corner-sharing OLi2MnP tetrahedra. In the thirty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted linear geometry to one Mn2+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a linear geometry to one V4+ and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the fortieth O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form a mixture of distorted edge and corner-sharing OLi2MnP tetrahedra. In the forty-first O2- site, O2- is bonded to two Li1+, one Mn2+, and one P5+ atom to form a mixture of distorted edge and corner-sharing OLi2MnP trigonal pyramids. In the forty-second O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V4+, and one P5+ atom. In